PDF of article. - Physics - Georgetown University

physica

pss

www.pss-b.com

status

solidi

basic solid state physics

b

Enhancement **of** thermoelectric performance

in strongly correlated multilayered nanostructures

J. K. Freericks 1 and V. Zlatić 2

1

Department **of** **Physics**, **Georgetown** **University**, Washington, DC 20057, USA

2

Institute **of** **Physics**, Zagreb, Croatia

Received 9 September 2006, accepted 21 September 2006

Published online 17 April 2007

PACS 71.27.+a, 71.30.+h, 73.20.–r, 73.40.Rw

We illustrate how the electronic charge reconstruction near the interfaces **of** metal–strongly-correlatedbarrier–metal

devices can lead to a significant enhancement **of** the thermoelectric response due to the

breaking **of** p**article**-hole symmetry. We show how one can achieve effective Seebeck coefficients larger

than 150 µV/K and effective electronic figures-**of**-merit ZT higher than 1. Our work shows that electronic

thermoelectric transport properties can be significantly enhanced from inhomogeneities created by the rearrangement

**of** charge near the interfaces, and that bulk figures-**of**-merit cannot generically be employed

to determine the figure-**of**-merit **of** a multilayered nanostructure.

phys. stat. sol. (b) 244, No. 7, 2351–2356 (2007) / DOI 10.1002/pssb.200674611

REPRINT

Original

Paper

phys. stat. sol. (b) 244, No. 7, 2351–2356 (2007) / DOI 10.1002/pssb.200674611

Enhancement **of** thermoelectric performance

in strongly correlated multilayered nanostructures

J. K. Freericks *, 1 and V. Zlatić **, 2

1

2

Department **of** **Physics**, **Georgetown** **University**, Washington, DC 20057, USA

Institute **of** **Physics**, Zagreb, Croatia

Received 9 September 2006, accepted 21 September 2006

Published online 17 April 2007

PACS 71.27.+a, 71.30.+h, 73.20.–r, 73.40.Rw

We illustrate how the electronic charge reconstruction near the interfaces **of** metal–strongly-correlatedbarrier–metal

devices can lead to a significant enhancement **of** the thermoelectric response due to the

breaking **of** p**article**-hole symmetry. We show how one can achieve effective Seebeck coefficients larger

than 150 µV/K and effective electronic figures-**of**-merit ZT higher than 1. Our work shows that electronic

thermoelectric transport properties can be significantly enhanced from inhomogeneities created by the rearrangement

**of** charge near the interfaces, and that bulk figures-**of**-merit cannot generically be employed

to determine the figure-**of**-merit **of** a multilayered nanostructure.

© 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim

1 Introduction

Seebeck and Peltier discovered two different thermoelectric effects in the early 1800s: Seebeck [1] discovered

that when two metals are joined together and placed in a thermal gradient, that a voltage develops,

while Peltier [2] found that electrons moving through a material carry both charge and heat. These

effects are generically small – a temperature difference **of** 10 K will yield a voltage difference **of**

10 - 100 µV in ordinary metals. Doped semiconductors were recognized to be good candidate materials

for thermoelectric effects in the 1950s [3], and a significant period **of** research activity took place to

optimize their properties resulting in the discovery **of** Bi–Te–Sb alloys, which are used in most commercial

devices for refrigeration and power generation. Nevertheless, thermoelectric power generation

and refrigeration remains a niche market, where the reliability, durability, and the vibration isolation **of**

the devices are more important than their efficiency; thermoelectric devices typically operate at a small

fraction **of** the maximal allowed Carnot efficiency.

The usefulness **of** a bulk material for deployment in a thermoelectric device is summarized by the socalled

figure-**of**-merit ZT = σS 2 T/

κ, where σ is the dc conductivity, S is the Seebeck coefficient, T is

the temperature, and κ is the thermal conductivity. The best materials used in thermoelectric devices

have ZT values near 1 [4]. Some new materials have been found that have ZT values near 2 [5], but they

have not yet been commercialized. If ZT could be increased to 4, refrigerators would have similar efficiency

to conventional coolant-based refrigerators, and power generators would become competitive

with steam turbines. While there is no theoretical maximum to the figure-**of**-merit, it has proved to be

difficult to find ways to increase its magnitude. This is because an increase in the conductivity usually

leads to a corresponding increase in the thermal conductivity, and the thermopower is not easy to tune.

* Corresponding author: http://www.physics.georgetown.edu/~jkf, Phone: + 202 687 6179, Fax: + 202 687 2087

** http://www.ifs.hr/~zlatic

© 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim

2352 J. K. Freericks and V. Zlatić: Enhancement **of** thermoelectric performance

Since the thermal conductivity includes both electronic and phononic pieces, much work in enhancing

the figure-**of**-merit has focused on finding ways to reduce the phonon contribution to the thermal conductivity,

but leaving the electronic transport unchanged. This electron-crystal–phonon-glass approach [6]

has been used by introducing rattling modes into skudderudites or clathrates or by introducing phonon

scattering via multilayered interfaces with widths on the order **of** nms [7].

In this work, we take a different approach, and examine whether one can enhance the electronic contributions

to thermoelectric phenomena by creating appropriate multilayered nanostructures. As an example,

we consider a p**article**-hole symmetric (half-filled) ballistic metal for the leads **of** the device, with

a barrier that is a p**article**-hole symmetric Mott insulator. Since both pieces **of** the device are p**article**-hole

symmetric, they are thermoelectrically inert, with S = 0 in the bulk. If the chemical potentials **of** the two

materials do not match, then there will be an electronic charge reconstruction that will break the overall

p**article**-hole symmetry **of** the device, and allow it to have a thermoelectric response. If we can tune the

electrochemical potential that arises from the rearrangement **of** charge in such a way, that it lies close to

the upper or lower Hubbard band edges, then we have a near-optimal situation for enhancing the Seebeck

coefficient, since the local density **of** states will be quite asymmetric. This procedure works remarkably

well, as described below, and it opens the door to a new strategy for enhancing the thermoelectric performance

**of** devices. Since the multilayered structures should also reduce the phonon thermal conductivity,

due to additional interface scattering, one expects these systems to be able to work quite well as

thermoelectric elements.

2 Formalism

The many-body formalism for solving the inhomogeneous dynamical mean-field theory **of** a multilayered

nanostructure is complex, and cannot be derived in detail here. Instead, we will describe the basic

ideas, and refer to other publications where detailed derivations can be found [8–11].

The systems we wish to model are composed **of** ballistic metal leads (no scattering whatsoever) which

surround a strongly correlated barrier region. For simplicity, we take the lattice sites to lie at the positions

**of** a simple cubic lattice, and we assume the same hopping between any two lattice sites (both interplane

and intraplane). Inhomogeneity is allowed only in the longitudinal (z ) direction, where the

planes can be described by different models. In the leads, we simply take a tight-binding single-band

model on a semi-infinite simple cubic lattice at half filling µ = 0, while the barrier is described by the

Falicov–Kimball model [12] at half filling for both the mobile and localized p**article**s; in the Falicov–

Kimball model mobile electrons are described by a tight-binding model but they also interact with localized

p**article**s with an interaction strength U (we choose the spinless version **of** the model). In the bulk,

the Falicov-Kimball model on a simple cubic lattice has a Mott metal-insulator transition at U ª 49 . t,

where t is the nearest-neighbor hopping integral. For concreteness we will measure all energies in units

**of** t, and we will set t = 025 . eV, which corresponds to a bare bandwidth **of** 3 eV.

In the bulk, both the ballistic metal leads and the Falicov–Kimball model barrier have vanishing Seebeck

coefficient S = 0, because they are p**article**-hole symmetric. Hence they have no thermoelectric

response. Our idea is to imagine that the chemical potential **of** the barrier is mismatched with that **of** the

metal leads by an amount denoted D Ef

(because the metal leads extend to infinity in each direction, they

determine the chemical potential **of** the device). As we shift the band **of** the barrier upwards in energy,

we break the p**article**-hole symmetry **of** the system, and allow it to have a thermoelectric response (the

parameter D Ef

is added to the chemical potential on each plane). Because the bulk Mott insulator has a

well defined gap, if we can tune the density **of** states **of** the barrier to lie right at the upper band edge **of**

the lower Hubbard band, or the lower band edge **of** the upper Hubbard band, then we have an opportunity

for a large thermoelectric response because we are maximizing the p**article**-hole asymmetry. Furthermore,

as we have DOS near the chemical potential, the system is likely to display metallic characteristics

rather than insulating ones, so it is possible that the phonon contribution to the thermal conductivity

will not overwhelm the electronic contribution, and the electronic estimate **of** the figure **of** merit may be

close to the actual value that can be achieved in devices.

© 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim www.pss-b.com

Original

Paper

phys. stat. sol. (b) 244, No. 7 (2007) 2353

This description has so far ignored the notion **of** electronic charge reconstruction, which plays an

important role in these devices [10, 13, 14]. If the barrier is not located at its bulk chemical potential,

electrons will spill out **of** or into the barrier. This will create a screened dipole layer at each metal-barrier

interface, which will ultimately determine the total number **of** electrons transfered. The rearrangement **of**

charge also creates an electrical potential energy, which must be included in the many-body theory.

Finally, we need to be able to calculate the charge and heat transport, which can be done by using a realspace

version **of** the Kubo formula [15, 16] (it must be in real space because the system lacks translational

invariance along the longitudinal direction). These transport coefficients can be determined by utilizing the

Jonson–Mahan theorem [10, 11, 17] in a real-space format. Details for how to do so appear elsewhere.

We find the Green’s functions and the self-energies from a self-consistent iterative approach to inhomogeneous

dynamical mean-field theory with the Potth**of**f–Nolting algorithm [8]. The electronic charge reconstruction

is determined in a semiclassical fashion, where the Coulomb potential energy is found from a

classical solution **of** Poisson’s equation, and this then determines the electrochemical potential on each

plane, which is input into the inhomogeneous dynamical mean-field theory to find the electron charge on

each plane. Solving these problems self-consistently is much more difficult than when there is no charge

8

reconstruction, and we typically need 3000–6000 iterations to reach a convergence **of** one part in 10 .

3 Numerical results

In Fig. 1, we plot false-color plots **of** the local electronic density **of** states for different planes as a function

**of** frequency (horizontal axis). We take 30 self-consistent planes in each metal lead, which are cou-

Fig. 1 (online colour at: www.pss-b.com) Density **of**

states for half **of** the nanostructure in a false color plot; top

panel is for D Ef = 0, middle for D Ef = - 1 and bottom for

D E f = - 3. Note how the mismatch **of** the chemical potentials

makes the bands more and more asymmetric, but how

the center **of** the barrier lies close to the p**article**-hole

symmetric case.

www.pss-b.com

© 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim

2354 J. K. Freericks and V. Zlatić: Enhancement **of** thermoelectric performance

Fig. 2 (online colour at: www.pss-b.com) (a) Electronic charge reconstruction and (b) potential at

T = 300 K for various D Ef

values. Note the similarity in shape **of** the charge pr**of**iles, and how the potential

energy increases in magnitude as the mismatch increases.

pled to bulk metal to make the semi-infinite lead, and the barrier region is 20 atomic planes thick. Since

the device is mirror symmetric, we show only half **of** the device, with the metal leads lying to the upper

part **of** the figure and the barrier to the bottom. Panel (a) is for the p**article**-hole symmetric case where the

chemical potentials match at all T . The barrier is described by a Mott insulator with U = 6, which creates

a gap **of** about 200 meV and a barrier height **of** about 100 meV. Note how the density **of** states has a deep

trench near zero frequency, and how the presence **of** the barrier introduces Friedel-like oscillations

within the density **of** states **of** the metal lead. In Panel (b), we have a shift **of** the chemical potentials by

one unit D Ef = - 1 and in panel (c) the shift is 3 units D Ef = - 3. Note how the density **of** states becomes

asymmetric due to the shifts, and how the Coulomb potential energy tends to bring the central planes **of**

the barrier closer to the chemical potential **of** the leads.

In Fig. 2, we plot the electronic charge pr**of**ile and potential energy at T = 300 K for various chemical

potential mismatches. We choose the effective dielectric constant so that the screening length for the

charge rearrangement is on the order **of** two lattice spacings. Note how the size **of** the charge rearrangement

grows with the mismatch [panel(a)], but appears to have the same shape for the different cases. The

electronic potential energy grows with the mismatch as expected, but the maximal magnitude **of** the

potential energy (at the center **of** the barrier) is always smaller in magnitude than the mismatch.

In Fig. 3, we show the temperature dependence **of** the charge pr**of**ile and the potential energy for

D E f = - 05 . . Note how the system has a substantial temperature dependence even at relatively low temperatures.

This illustrates the importance **of** self-consistently solving for the electronic charge reconstruction

at each temperature. It also shows that the temperature evolution **of** these devices may produce dif-

Fig. 3 (online colour at: www.pss-b.com) (a) Electronic charge reconstruction and (b) potential at

D E f = - 05 . for various temperatures values. Note how the charge rearrangement can depend strongly on

the temperature.

© 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim www.pss-b.com

Original

Paper

phys. stat. sol. (b) 244, No. 7 (2007) 2355

Fig. 4 (online colour at: www.pss-b.com) (a)

Seebeck coefficient, (b) Lorenz number, and (c)

figure-**of**-merit versus temperature for various D Ef

values. The figure **of** merit is highest at low temperatures

for moderate chemical potential mismatches.

As the mismatch grows, the peak maximum

drops, and moves to higher temperature.

ferent behavior than seen in bulk systems, because there is this additional temperature dependence to the

“scattering potential”.

The main results for the thermoelectric transport are shown in Fig. 4. We plot the Seebeck coefficient

in panel (a). Note how the peak is reduced in magnitude, and moves to higher energies as the

mismatch is increased. In metallic systems, achieving a Seebeck coefficient larger than 156 µV/K will

create a figure-**of**-merit larger than 1. Here we can get large Seebeck coefficients in numerous different

temperature ranges simply by tuning the chemical potential mismatch. The effective Lorenz number

[18] satisfies L = R/

( RthT)

, using the resistance R **of** the junction, the thermal resistance R th and

2

the temperature T . In a metallic system at low temperature, the Lorenz number is equal to π / 3. In all

cases we consider, we see this result, although the temperature dependence **of** the Lorenz number can

be significant. In cases where it dips below π 2 / 3, which occurs for all systems for some temperature

range, the thermoelectric properties can be enhanced. When it becomes larger, the thermoelectric

2

properties are degraded. In panel (c), we plot an effective device ZT = S /L. Note how there is a robust

low-temperature region where ZT is larger than one. As the mismatch increases in magnitude, the

ZT value has its maximum pushed to higher T , but it also has its maximum value lowered. This tracks

most closely with the behavior **of** the Seebeck coefficient.

The reason why we see a maximum to the Seebeck coefficient (as a function **of** the chemical potential

mismatch), is because the band edge for the Mott insulator moves continuously with the chemical potential

mismatch (and it approaches a fixed location deep within the barrier). The band edge passes by the

chemical potential close to the D Ef = - 025 . case, which is why it has such a large thermoelectric response.

As D Ef

becomes more negative, the response gets reduced, as we expect. As D Ef

approaches

zero, we can find very large Seebeck coefficients and ZT values, which occur at lower and lower temperatures.

But the conductances are so low, that it becomes a bad approximation to neglect the phonon

thermal conductance, and the actual figure-**of**-merit is probably reduced significantly. Of course, when

D E f = 0, the Seebeck coefficient and ZT both vanish for all T .

www.pss-b.com

© 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim

2356 J. K. Freericks and V. Zlatić: Enhancement **of** thermoelectric performance

4 Conclusions

In this work, we have considered the thermal transport when two bulk materials, both with vanishing

Seebeck and Peltier coefficients, are joined in a sandwich structure to create a device. Because the

chemical potentials **of** the materials do not generically match, there is an electronic charge reconstruction,

which breaks the p**article**-hole symmetry **of** the system and creates a thermoelectric response. Surprisingly,

if the barrier material is a small-gap Mott insulator, one can generate a significant effect, if the

bands are tuned so that the electrochemical potential lies close to one **of** the strongly correlated electron

band edges. Indeed, we can easily generate electronic figures **of** merit larger than 1 over fairly wide temperature

ranges. As the mismatch **of** the bands increases further, the effect is pushed to higher temperatures,

but tends to shrink in overall magnitude.

There are two important comments to make about this work. First, we have only calculated the electronic

contribution to the thermoelectric figure-**of**-merit. If the thermal conductance from the phonons is

large enough, the phonons can form a thermal short for the conduction **of** heat, which will dramatically

reduce the overall figure **of** merit by sharply increasing the total thermal conductance. As the devices

become more metallic, which occurs as the mismatch is made larger, this problem is reduced, because

the electronic contribution to the thermal conductance becomes important and can dominate the phonon

piece. Second, we have made no attempt to try to optimize the effect in terms **of** selection **of** materials

for the various parts **of** the device (which governs the interaction strength and the band mismatches) or

for the thicknesses **of** the different layers (which is how one tunes the effect for a given material), so it

may be possible that even larger enhancements can be found as the result **of** an optimization study.

Acknowledgement We acknowledge support from the National Science Foundation under grant number

DMR-0210717.

References

[1] T. J. Seebeck, Abh. Dtsch. Akad. Wiss. Berl. 265 (1823).

[2] J. C. A. Peltier, Ann. Chim. Phys. 56, 371 (1834).

[3] A. F. I**of**fe, Semiconductor thermoelectrics and thermoelectric cooling (Infosearch, London, 1957).

[4] G. D. Mahan, Solid State Phys. 51, 81 (1998).

[5] K. F. Hsu, S. Loo, F. Guo, W. Chen, J. S. Dyck, C. Uher, T. Hogan, E. K. Polychroniadis, and M. G. Kanatzidis,

Science 303, 818 (2004).

V. K. Zaitsev, M. I. Fedorov, E. A. Gurieva, I. S. Eremin, P. P. Konstantinov, A. Yu. Samunin, and M. V. Vedernikov,

Phys. Rev. B 74, 045207 (2006).

[6] G. A. Slack and V. Tsoukala, J. Appl. Phys. 76, 1665 (1994).

G. S. Nolas, J. Sharp, and J. Goldsmid, Thermoelectrics: basic principles and new materials (Springer-Verlag,

Berlin, 2001).

[7] L. D. Hicks and M. D. Dresselhaus, Phys. Rev. B 47, 12727 (1993).

R. Venkatasubramanian, E. Sivola, T. Colpitts, and B. O’Quinn, Nature (London) 413, 597 (2001).

[8] M. Potth**of**f and W. Nolting, Phys. Rev. B 59, 2549 (1999).

[9] J. K. Freericks, Phys. Rev. B 70, 195342 (2004).

[10] J. K. Freericks, Transport in multilayered nanostructures: the dynamical mean-field theory approach (Imperial

College Press, London, 2006).

[11] J. K. Freericks, V. Zlatić, and A. V. Shvaika, Phys. Rev. B 75, 035133 (2007).

[12] L. M. Falicov and J. C. Kimball, Phys. Rev. Lett. 22, 997 (1969).

[13] B. K. Nikolić, J. K. Freericks, and P. Miller, Phys. Rev. B 65, 064529 (2002).

[14] S. Okamoto and A. J. Millis, Nature (London) 428, 630 (2004).

[15] R. Kubo, J. Phys. Soc. Jpn. 12, 570 (1957).

[16] D. A. Greenwood, Proc. Phys. Soc. (London) 71, 585 (1958).

[17] M. Jonson and G. D. Mahan, Phys. Rev. B 21, 4223 (1980); Phys. Rev. B 42, 9350 (1990).

[18] L. Lorenz, Ann. Phys. Chem. (Leipzig) 147, 429 (1872).

© 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim www.pss-b.com